Mechanical Failure. Chapter 9. Overview. Failure Modes Fracture, Fatigue, Creep Fracture Modes Ductile, Brittle, Intergranular, Transgranular Fracture Toughness Stress Concentrators (Flaws) Crack Propagation. Fracture Modes.
Simple fracture is the separation of a body into 2 or more pieces in response to an applied stress that is static (constant) and at temperatures that are low relative to the Tm of the material.
Classification is based on the ability of a material to experience plastic deformation.
Accompanied by significant plastic deformation
Little or no plastic deformation
Imposed stress Crack Formation Propagation
Cracks propagate due to sharpness of crack tip
A plastic material deforms at the tip, “blunting” the crack.
Energy balance on the crack
Elastic strain energy-
energy stored in material as it is elastically deformed
this energy is released when the crack propagates
creation of new surfaces requires energy
%AR or %EL
• Ductile fracture is
usually more desirable
than brittle fracture.
Brittle: No warning
Warning before fracture
serve as void
From V.J. Colangelo and F.A. Heiser, Analysis of Metallurgical Failures (2nd ed.), Fig. 11.28, p. 294, John Wiley and Sons, Inc., 1987. (Orig. source: P. Thornton, J. Mater. Sci., Vol. 6, 1971, pp. 347-56.)
Fracture surface of tire cord wire loaded in tension. Courtesy of F. Roehrig, CC Technologies, Dublin, OH. Used with permission.
• Evolution to failure:
• Brittle failure:
-- many pieces
-- small deformations
• Ductile failure:
-- one piece
-- large deformation
Figures from V.J. Colangelo and F.A. Heiser, Analysis of Metallurgical Failures (2nd ed.), Fig. 4.1(a) and (b), p. 66 John Wiley and Sons, Inc., 1987. Used with permission.
Ductile vs. Brittle Failure
(a) SEM image showing spherical dimples resulting from a uniaxial tensile load. (b) SEM image of parabolic dimples from shear loading.
Arrows indicate point at failure origination
Distinctive pattern on the fracture surface: V-shaped “chevron” markings point to the failure origin.
Studies the relationships between:
Fracture toughness measures a material’s resistance to brittle fracture when a crack is present.
It is an indication of the amount of stress required to propagate a preexisting flaw.
Flaws may appear as cracks, voids, metallurgical inclusions, weld defects, design discontinuities, or some combination thereof.
It is common practice to assume that flaws are present and use the linear elastic fracture mechanics (LEFM) approach to design critical components.
This approach uses the flaw size and features, component geometry, loading conditions and the fracture toughness to evaluate the ability of a component containing a flaw to resist fracture.
The effect of a stress raiser is more significant in brittle than in ductile materials.
For a ductile material, plastic deformationresults when the maximumstress exceeds the yield strength.
This leads to a more uniform distribution of stress in the vicinity of the stress raiser; the maximum stress concentration factor will be less than the theoretical value.
In brittle materials, there is no redistribution or yielding.
K ≥ Kc
Stress Intensity Factor:
--Depends on load & geometry.
--Depends on the material,
temperature, environment &
rate of loading.
Fracture toughness - good diagrams
single edge notch bend (SENB or three-point bend)
If the crack is similar to an elliptical hole through plate, and is oriented perpendicular to applied stress, the maximum stress σm=
where t = radius of curvature
so = applied stress
sm = stress at crack tip
a = length of surface crack or ½ length of internal crack
sm /so = Ktthe stress concentration factor
K ≥ Kc
• Crack growth condition:
• Largest, most stressed cracks grow first.
--Result 2: Design stress
dictates max. flaw size.
--Result 1: Max flaw size
dictates design stress.
• Material has Kc = 26 MPa-m0.5
• Two designs to consider...
-- use same material
-- largest flaw is 4 mm
-- failure stress = ?
-- largest flaw is 9 mm
-- failure stress = 112 MPa
• Key point: Y and Kc are the same in both designs. Y is a dimensionless parameter; see Callister page 298.
• Reducing flaw size pays off.
Structural health monitoring (SHM) systems can be arrayed in similar fashion to the human nervous system, with sensors concentrated in key areas where loads are highest.
A piezoelectric-based sensor system from Acellent Technologies, called SMART Layer, identifies damage with small ceramic actuators
An FAA-sponsored study on curved honeycomb-cored panels showed that acoustic emission (AE) monitoring is a reliable method for locating damage initiation sites and for tracking crack progression. Source: Physical Acoustics Corp
A comparative vacuum-monitoring (CVM) sensor, is a thin, self-adhesive rubber patch that detects cracks in the underlying material. The rubber is laser-etched with rows of tiny, interconnected channels or galleries, to which an air pressure is applied. Any propagating crack under the sensor breaches the galleries and the resulting change in pressure is monitored.
Surface of a 6-mm diameter fused silica rod.
Characteristic fracture behavior in ceramics
Initial region (mirror) is flat and smooth
After reaches critical velocity crack branches
• Impact loading:
-- severe testing case
-- makes material more brittle
-- decreases toughness
• Pre-WWII: The Titanic
• WWII: Liberty ships
Disastrous consequences for a welded transport ship, suddenly split across the entire girth of the ship (40˚F). The vessels were constructed from steel alloys that exhibit a DBTT room temp
Reprinted w/ permission from R.W. Hertzberg, "Deformation and Fracture Mechanics of Engineering Materials", (4th ed.) Fig. 7.1(a), p. 262, John Wiley and Sons, Inc., 1996. (Orig. source: Dr. Robert D. Ballard, The Discovery of the Titanic.)
Charpy Impact Energy (A) and Shear Fracture % (B) Correlated with Temperaturec09f19
• Increasing temperature...
-- increases %EL and Kc
• Ductile-to-Brittle Transition Temperature (DBTT)...
FCC metals (e.g., Cu, Ni)
BCC metals (e.g., iron at T < 914°C)
High strength materials (
Fatigue testing apparatus for rotating bending test
Fatigue failure is brittle in nature, even in normally ductile materials; there is very little plastic deformation associated with the failure.
The image shows fatigue striations (microscopic).
• Crack grows incrementally
typ. 1 to 6
increase in crack length per loading cycle
• Failed rotating shaft
-- crack grew even though
Kmax < Kc
-- crack grows faster as
• Ds increases
• crack gets longer
• loading freq. increases.
Fig. 9.28, Callister & Rethwisch 3e. (Fig. 9.28 is from D.J. Wulpi, Understanding How Components Fail, American Society for Metals, Materials Park, OH, 1985.)
Creep strain vs time at constant load and constant elevated temperature. Minimum creep rate (steady-state creep rate), is the slope of the linear segment in the secondary region. Rupture lifetime tr is the total time to rupture.
• Strain rate
for higher T, s
Steady state creep rate (%/1000hr)
• Strain rate is constant at a given T, s
-- strain hardening is balanced by recovery
stress exponent (material parameter)
activation energy for creep
• Engineering materials don't reach theoretical strength.
• Flaws produce stress concentrations that cause
• Sharp corners produce large stress concentrations
and premature failure.
• Failure type depends on T and stress:
- for noncyclic s and T < 0.4Tm, failure stress decreases with:
- increased maximum flaw size,
- decreased T,
- increased rate of loading.
- for cyclic s:
- cycles to fail decreases as Ds increases.
- for higher T (T > 0.4Tm):
- time to fail decreases as s or T increases.